Journal of Chemistry
Volume 2017 (2017), Article ID 6836375, 8 pages
https://doi.org/10.1155/2017/6836375

Research Article

Synthesis of Gold Nanoparticles Stabilized in Dextran Solution by Gamma Co-60 Ray Irradiation and Preparation of Gold Nanoparticles/Dextran Powder

Phan Ha Nu Diem,1,2 Doan Thi Thu Thao,³ Dang Van Phu,⁴ Nguyen Ngoc Duy,⁴ Hoang Thi Dong Quy,³ Tran Thai Hoa,² and Nguyen Quoc Hien⁴

¹Dong Nai University, 4 Le Quy Don, Bien Hoa City, Vietnam
²College of Sciences, Hue University, 77 Nguyen Hue, Hue City, Vietnam
³University of Science, Vietnam National University in Ho Chi Minh City, 227 Nguyen Van Cu, Ho Chi Minh City, Vietnam
⁴Research and Development Center for Radiation Technology, Vietnam Atomic Energy Institute, 202A Street 11, Linh Xuan Ward, Thu Duc District, Ho Chi Minh City, Vietnam

Correspondence should be addressed to Nguyen Quoc Hien; hien7240238@yahoo.com

Received 7 August 2017; Accepted 17 September 2017; Published 16 October 2017

Academic Editor: Philippe Dugourd

Copyright © 2017 Phan Ha Nu Diem et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.

Abstract.

Gold nanoparticles (AuNPs) in spherical shape with diameter of 6–35 nm stabilized by dextran were synthesized by γ-irradiation method. The AuNPs were characterized by UV-Vis spectroscopy and transmission electron microscopy. The influence of pH, Au³⁺ concentration, and dextran concentration on the size of AuNPs was investigated. Results indicated that the smallest AuNPs size (6 nm) and the largest AuNPs size (35 nm) were obtained for pH of 1 mM Au³⁺/1% dextran solution of 5.5 and 7.5, respectively. The smaller Au³⁺ concentration favored smaller size and conversely the smaller dextran concentration favored bigger size of AuNPs. AuNPs powders were prepared by spay drying, coagulation, and centrifugation and their sizes were also evaluated. The purity of prepared AuNPs powders was also examined by energy dispersive X-ray (EDX) analysis. Thus, the as-prepared AuNPs stabilized by biocompatible dextran in solution and/or in powder form can be potentially applied in biomedicine and pharmaceutics.

1. Introduction

Synthetic polymers typically polyvinyl alcohol [1], polyvinyl pyrrolidone [2, 3], polyethylene glycol [4], sodium polyacrylate [5, 6], and surfactants [7, 8] have been commonly used as stabilizers in the bottom-up approach of synthesis of gold nanoparticles (AuNPs). In addition, biopolymers such as chitosan [9–11], alginate [12, 13], hyaluronan [14, 15], gum arabic [16, 17], protein [18, 19], gelatin [20], dextran [21], and glucomannan [22] have been also used as stabilizers of colloidal AuNPs solution. On the other hand, materials based on functionalized AuNPs are regarded as one of the most important nanocomposites especially due to their biological and catalytic activities [23, 24]. For example, assembly of chromanol group on AuNPs could efficiently enhance the activity of the vitamin E-derived antioxidant [25]; aptamer-conjugated AuNPs showed the advantages in detection of cancer cells by colorimetric assay [26], AuNPs supported on MgO for CO oxidation [27].

Various methods for the synthesis of AuNPs through bottom-up approach, that is, reduction of Au³⁺ ions in solution, have been reported [11] and the most common method is chemical reduction of gold salt precursor using chemical reducing agents. Compared with other methods, gamma Co-60 ray irradiation has been considered as an effective method with several advantages as described by Hien et al. [15]. In addition, gamma Co-60 ray irradiation has been also considered as a green method to noble metal nanoparticle synthesis [28]. Dextran polysaccharide composed of repeated monomeric glucose units with a predominance of 1,6-α-D-glucopyranosyl linkages and annual world production is of about 500 metric tons [29]. Dextran is readily soluble in water and electrolytes with excellent stability and it has wide range of use in food, medical related areas, and biological functions, especially for blood flow improvement by reduction of blood viscosity and inhibition of erythrocyte aggregation [30, 31]. Therefore, dextran stabilized AuNPs are promising to use for intravenous administration as X-ray contrast agent [16, 32], cancer therapy [33, 34] including photothermal cancer therapy [35, 36], and for other purposes of application as well [23].

In the present study, AuNPs were synthesized by gamma Co-60 ray irradiation method using dextran as stabilizer and hydroxyl radical () scavenger. The influence of pH, Au³⁺ and dextran concentrations in aqueous solution on the size of AuNPs was studied. AuNPs powders from AuNPs/dextran solution were prepared by spray drying, coagulation, and centrifugation methods. The purity and size of the AuNPs powders were also examined.

2. Experiments

2.1. Materials and Chemicals

Hydrogen tetrachloroaurate trihydrate (HAuCl₄·3H₂O) was obtained from Merck, Germany. Dextran (MW 60,000–90,000) was purchased from Himedia, India. Other chemicals were of analytical grade and used as received. Distilled water was used in all experiments. Glassware was treated with regia solution (1V HNO₃ : 3V HCl), washed with distilled water, and dried.

2.2. Preparation of Au³⁺/Dextran Solution and γ-Irradiation

Two stock solutions particularly 10 mM Au³⁺ and 4% dextran were prepared by dissolving HAuCl₄·3H₂O and dextran into water. Au³⁺/dextran solutions were prepared by pouring Au³⁺ solution into dextran solution with desired different concentration while stirring for about 10 min. pH of Au³⁺/dextran solution was adjusted to 5.5, 6.5, and 7.5 by 0.5% NH₄OH solution. Then, the prepared Au³⁺/dextran solutions of 100 ml were put into glass bottles with plastic cap. Irradiation of Au³⁺/dextran solutions was carried out on the gamma Co-60 irradiator SVST Co-60/B (Hungary) with dose rate of 1.1 kGy/h at VINAGAMMA Center, Ho Chi Minh City, at ambient condition with required doses (~6 kGy for reduction of 1 mM Au³⁺) as reported in our previous paper [15].

2.3. Characterization of AuNPs/Dextran

The absorption spectra of AuNPs/dextran solutions obtained after γ-irradiation were taken on an UV-Vis spectrophotometer model UV-2401PC (Shimadzu, Japan). The size and size distribution of the AuNPs were characterized from TEM images on transmission electron microscope (TEM) model JEM1010 (JEOL, Japan) and statistically calculated from about 300 particles. The AuNPs/dextran solution from 1 mM Au³⁺/1% dextran sample was used to prepare AuNPs powder by spray drying on spray dryer model ADL311 (Yamato, Japan) and by centrifugation on ultra centrifuged machine model Ultra 5.0 (Hanil Science Industrial, Korea) at 30,000 rpm for 20 min. After centrifugation, the AuNPs precipitate was isolated and dried in forced air oven (DNF 410, Yamato, Japan) at 60°C. The AuNPs powder was also prepared by coagulation with solvent mixture of ethanol/acetone with equal volume ratio. For coagulation of AuNPs/dextran, 8 volumes of solvent mixture were used to mix with 1 volume of AuNPs/dextran solution. The resulting AuNPs/dextran coagulate was filtered and washed several times with solvent and dried in forced air oven at 60°C. The purity of AuNPs/dextran powders was assessed by energy dispersive X-ray spectroscopy (EDX) on a JEOL 6610 LA. The UV-Vis spectra and TEM images of AuNPs powders redissolved in water were also taken.

3. Results and Discussions

After irradiation, the color of Au³⁺/dextran solution turned from yellow to ruby-red which is surface plasmon resonance characterized for AuNPs [11, 15]. The mechanism of reduction of Au³⁺ to Au° by γ-irradiation method through the reducing species which resulted from water radiolysis was described by Henglein [1].

3.1. Effect of pH

Results of UV-Vis spectra in Figure 1 indicated that the maximum absorption wavelengths () of AuNPs/dextran solutions were of 543.5, 526.0, and 520.5 nm for pH 5.5, 6.5, and 7.5, respectively.

Figure 1: UV-Vis spectra of 1 mM AuNPs/1% dextran solutions at different pH: 5.5 (a), 6.5 (b), and 7.5 (c).

Results of TEM images and size distribution histograms in Figure 2 indicated that the size of AuNPs decreased with the increase of pH value and particularly the particle sizes were of 35.5, 24.1, and 6.2 nm for pH 5.5, 6.5, and 7.5, respectively. It is clear that slightly basic medium (pH 7.5) was a suitable condition to synthesize AuNPs stabilized by dextran with smaller size (6.2 nm) and narrower particles size distribution (Figures 2(C) and 2(c)) compared to lower pH (6.5) (Figures 2(B) and 2(b)) or acidic medium pH 5.5 (Figures 2(A) and 2(a)) by γ-irradiation method. The obtained results suggested that adjustment of pH of Au³⁺/dextran solution before irradiation significantly affected the size of AuNPs. The same results of the pH effect were also reported by Phu et al. on radiolytic synthesis of AgNPs stabilized by chitosan [37]. Particularly, the sizes of AgNPs were of 15.0 and 7.3 nm for pH 3 and 6, respectively.

Figure 2: TEM images and size distribution histograms of AuNPs/dextran at different pH: 5.5 (A, a), 6.5 (B, b), and 7.5 (C, c).

3.2. Effect of Au³⁺ Concentration

In this experiment, AuNPs were synthesized from Au³⁺/detxran solutions containing 1% (w/v) dextran with various Au³⁺ concentrations particularly 0.5, 1.0, and 2.0 mM. The pH of Au³⁺/dextran solutions was adjusted to 7.5. The UV-Vis spectra in Figure 3 showed the at 519.5, 520.5, and 524.0 nm for Au³⁺ concentration of 0.5, 1.0, and 2.0 mM, respectively.

Figure 3: UV-Vis spectra of AuNPs/dextran solutions with various Au³⁺ concentrations: 0.5 (a), 1.0 (b), and 2.0 mM (c).

The TEM images and the size distribution histograms of the three AuNPs/dextran solutions with various Au³⁺ concentrations were shown in Figure 4. The sizes of AuNPs were of 5.8, 6.3, and 11.9 nm for Au³⁺ concentrations of 0.5, 1.0, and 2.0 mM, respectively. Thus, as Au³⁺ concentration increased the sizes of the AuNPs were bigger and shifted to longer wavelengths. The increase of AuNPs size with the increasing of Au³⁺ concentration was also reported in previous articles for AuNPs/PVP [3], AuNPs/alginate [13], and AuNPs/hyaluronan [15]. The reason for this phenomenon may be due to the development of clusters and the agglomeration among AuNPs when the ratio of stabilizer and Au³⁺ concentration is not high enough [15].

Figure 4: TEM images and size distribution histograms of AuNPs/dextran at various Au³⁺ concentrations: 0.5 (A, a), 1.0 (B, b), and 2.0 mM (C, c).

3.3. Effect of Dextran Concentration

In this experiment, the Au³⁺ concentration was fixed at 1 mM while the dextran concentrations were of 0.5, 1.0, and 2.0% (w/v) and the pH of Au³⁺/dextran solutions was also adjusted to 7.5. Results of UV-Vis spectra in Figure 5 showed at 522.5, 520.5, and 519.0 nm for the dextran concentrations of 0.5, 1.0, and 2.0%, respectively.

Figure 5: UV-Vis spectra of AuNPs/dextran solutions from different dextran concentrations: 0.5 (a), 1.0 (b), and 2.0% (c).

The sizes of AuNPs decreased with the increase of dextran concentration particularly the sizes of 8.0, 6.2, and 5.2 nm for dextran concentrations of 0.5, 1.0, and 2.0%, respectively (Figure 6). Thus, the decrease in the size of AuNPs was not much significant as the increase of dextran concentration from 0.5 to 2.0%.

Figure 6: TEM images and size distribution histogram of AuNPs/dextran at different dextran concentrations: 0.5 (A, a), 1.0 (B, b), and 2.0% (C, c).

Dextran has good ability to stabilize AuNPs due to the chain of dextran which consists of –OH and –COR groups which stabilize AuNPs thought steric and electrostatic effects [38]. Simultaneously, dextran acted as free radical scavenger via hydrogen abstraction by and released during radiolysis of water [11, 13, 15]. Therefore, scavenger such as alcohols is not necessary to add into Au³⁺/dextran solution as in the case of Au³⁺/PVP to prepare colloidal AuNPs solution by γ-irradiation method [3]. As described by Hien et al. [15], mass production of colloidal AuNPs solution can be suitably carried out by gamma Co-60 ray irradiation method. The production rate () of a gamma Co-60 irradiator can be calculated by (1) [39] as follows:

where is the absorbed dose (kGy), is the radiation energy utilization efficiency, and is source power (kW) (100 kCi is equivalent to 1.48 kW).

Assuming that one gamma Co-60 irradiator with activity of 300 kCi (eqv. 4.44 kW) is used for irradiation of Au³⁺/dextran solution with Au³⁺ concentration of 1 mM, at dose of 6 kGy and with , then the production rate of AuNPs/dextran solution calculated according to (1) will be of 932 kg/h (~932 litters/h). Besides mass production, the obtained colloidal AuNPs solution is of high purity without residues of excessive chemical reductant and by-products from chemical reductant after reduction process that were typically analyzed for using trisodium citrate as reducing agent [40].

3.4. Characteristics of AuNPs Powders

Photograph of AuNPs/dextran solution and powders was presented in Figure 7. The AuNPs powders are brownish-pink to dark-brownish in color depending on the powdering method.

Figure 7: Photograph of AuNPs/dextran solution (a), spray drying (b), coagulation (c), and centrifugation (d) of AuNPs powders.

Figure 8 presented the UV-Vis spectra of original AuNPs/dextran solution and AuNPs solutions from AuNPs powders. The values of and the sizes of AuNPs were shown in Table 1.

Table 1: The values of and the size of AuNPs () from AuNPs/dextran solution and powders prepared by different methods.

AuNPs sample
, nm
, nm

Solution
520.5
6.2 ± 0.4

Spray drying
522.0
7.5 ± 0.5

Coagulation
522.5
8.0 ± 0.3

Centrifugation
523.5
11.2 ± 0.5

Figure 8: UV-Vis spectra of original AuNPs/dextran solution (a), and AuNPs/dextran solutions from AuNPs/dextran powders: spray drying (b), centrifugation (c), and coagulation (d).

It is interesting to note that the value of and the size of AuNPs powders made from spray drying and coagulation were almost not much changed in comparison with those of original AuNPs/dextran solution, but these parameters increased for the AuNPs made from centrifugation (Table 1). The reason may be due to aggregation of AuNPs which occurred during centrifugation with ultrahigh speed (30,000 rpm). To the best of our knowledge, no research of the effect of AuNPs powder preparation methods on the characteristics of AuNPs, particularly and the size, has been reported yet except the study of the purity of AuNPs synthesized by using trisodium citrate as reducing agent and purified by centrifugation method which was reported [40]. Nevertheless, the final form of AuNPs in this study was not powder but referred to as “treated AuNPs suspension.”

Results of the EDX spectra in Figure 9 indicated that the AuNPs powders prepared by coagulation and centrifugation did not contain chlorine (Figures 9(b) and 9(c)); however the AuNPs powder prepared by spray drying was contaminated by 5.7% chlorine (Figure 9(a)). Thus, it can be deduced that AuNPs powders prepared by coagulation and centrifugation were of high purity. In other words, the AuNPs/dextran powders obtained by coagulation and centrifugation methods were effectively purified. However, chlorine content in AuNPs powder should be analyzed with more precise methods.

(a)

(b)

(c)

Figure 9: EDX spectra of AuNPs/dextran powders: spray drying (a), coagulation (b), and centrifugation (c).

The stability of colloidal AuNPs solution depends on various factors such as pH, dielectric constant, and concentration of ligand around the particles [19]. Furthermore, the stability of colloidal AuNPs solution stored at low temperature is better than at high ones [40]. In general, polysaccharides such as chitosan, hyaluronan, alginate, and dextran with oxygen rich structures in hydroxyl and ether groups lead to tightly binding polysaccharides to nanoparticles via steric and electrostatic interaction [38]. However, for a long time of storage, the AuNPs in colloidal AuNPs solution will be gradually aggregated to form bigger sizes due to sedimentation phenomenon of AuNPs in colloidal system. In addition, storage and transportation of colloidal AuNPs solution are not always convenient. In fact, it was observed that several samples of the synthesized AuNPs/dextran solutions stored at normal condition were randomly attacked by fungi. Therefore, in those aspects AuNPs powder is much more suitable. Besides, AuNPs/dextran powder holds great potential for biomedical and pharmaceutical applications; especially those AuNPs/dextran powders can be sterilized suitably by radiation method (gamma Co-60 ray, electron beam) [41] for use in intravenous administration for X-ray contrast imaging, photothermal cancer therapy, and in other purposes of application as well.

4. Conclusions

Dextran stabilized AuNPs with diameter in the range of 6–35 nm were synthesized by gamma Co-60 ray irradiation of Au³⁺ in dextran solution. The gamma Co-60 ray irradiation method for production of AuNPs can be favorably carried out on large scale. The AuNPs sizes can be controlled by varying pH, Au³⁺, and dextran concentrations. AuNPs powders with the almost unchanged size were also prepared by spray drying, coagulation, and centrifugation methods. Due to the biocompatibility of dextran, the purity of AuNPs/dextran colloidal solution as well as the AuNPs/dextran powders and unique attributes of AuNPs, AuNPs/dextran can be potentially applied in biomedicine and pharmaceutics especially in X-ray contrast imaging and photothermal cancer therapy.

Conflicts of Interest

The authors declare that they have no conflicts of interest.

Acknowledgments

This research is funded by Vietnam National Foundation for Science and Technology Development (NAFOSTED) under Grant no. “104.06-2014.87.”

References

A. Henglein, “Radiolytic preparation of ultrafine colloidal gold particles in aqueous solution: Optical spectrum, controlled growth, and some chemical reactions,” Langmuir, vol. 15, no. 20, pp. 6738–6744, 1999.

R. Seoudi, A. A. Fouda, and D. A. Elmenshawy, “Synthesis, characterization and vibrational spectroscopic studies of different particle size of gold nanoparticle capped with polyvinylpyrrolidone,” Physica B: Condensed Matter, vol. 405, no. 3, pp. 906–911, 2010.

T. Li, H. G. Park, and S.-H. Choi, “γ-Irradiation-induced preparation of Ag and Au nanoparticles and their characterizations,” Materials Chemistry and Physics, vol. 105, no. 2-3, pp. 325–330, 2007.

G. Zhang, Z. Yang, W. Lu et al., “Influence of anchoring ligands and particle size on the colloidal stability and in vivo biodistribution of polyethylene glycol-coated gold nanoparticles in tumor-xenografted mice,” Biomaterials, vol. 30, no. 10, pp. 1928–1936, 2009.

J. Belloni, M. Mostafavi, H. Remita, J.-L. Marignier, and M.-O. Delcourt, “Radiation-induced synthesis of mono- and multi-metallic clusters and nanocolloids,” New Journal of Chemistry, vol. 22, no. 11, pp. 1239–1255, 1998.

I. Hussain, M. Brust, A. J. Papworth, and A. I. Cooper, “Preparation of acrylate-stabilized gold and silver hydrosols and gold-polymer composite films,” Langmuir, vol. 19, no. 11, pp. 4831–4835, 2003.

T. K. Sau, A. Pal, N. R. Jana, Z. L. Wang, and T. Pal, “Size controlled synthesis of gold nanoparticles using photochemically prepared seed particles,” Journal of Nanoparticle Research, vol. 3, no. 4, pp. 257–261, 2001.

J. Duy, L. B. Connell, W. Eck, S. D. Collins, and R. L. Smith, “Preparation of surfactant-stabilized gold nanoparticle-peptide nucleic acid conjugates,” Journal of Nanoparticle Research, vol. 12, no. 7, pp. 2363–2369, 2010.

D. R. Bhumkar, H. M. Joshi, M. Sastry, and V. B. Pokharkar, “Chitosan reduced gold nanoparticles as novel carriers for transmucosal delivery of insulin,” Pharmaceutical Research, vol. 24, no. 8, pp. 1415–1426, 2007.

C. Sun, R. Qu, H. Chen et al., “Degradation behavior of chitosan chains in the 'green' synthesis of gold nanoparticles,” Carbohydrate Research, vol. 343, no. 15, pp. 2595–2599, 2008.

N. N. Duy, D. X. Du, D. Van Phu, L. A. Quoc, B. D. Du, and N. Q. Hien, “Synthesis of gold nanoparticles with seed enlargement size by γ-irradiation and investigation of antioxidant activity,” Colloids and Surfaces A: Physicochemical and Engineering Aspects, vol. 436, pp. 633–638, 2013.

G. Sonavane, K. Tomoda, and K. Makino, “Biodistribution of colloidal gold nanoparticles after intravenous administration: effect of particle size,” Colloids and Surfaces B: Biointerfaces, vol. 66, no. 2, pp. 274–280, 2008.

N. Tue Anh, D. Van Phu, N. Ngoc Duy, B. Duy Du, and N. Quoc Hien, “Synthesis of alginate stabilized gold nanoparticles by γ-irradiation with controllable size using different Au3+ concentration and seed particles enlargement,” Radiation Physics and Chemistry, vol. 79, no. 4, pp. 405–408, 2010.

H. Lee, K. Lee, I. K. Kim, and T. G. Park, “Synthesis, characterization, and in vivo diagnostic applications of hyaluronic acid immobilized gold nanoprobes,” Biomaterials, vol. 29, no. 35, pp. 4709–4718, 2008.

N. Q. Hien, D. Van Phu, N. N. Duy, and L. A. Quoc, “Radiation synthesis and characterization of hyaluronan capped gold nanoparticles,” Carbohydrate Polymers, vol. 89, no. 2, pp. 537–541, 2012.

V. Kattumuri, K. Katti, and S. Bhaskaran, “Gum arabic as a phytochemical construct for the stabilization of gold nanoparticles: in vivo pharmacokinetics and X-ray-contrast-imaging studies,” Small, vol. 3, no. 2, pp. 333–341, 2007.

C.-C. Wu and D.-H. Chen, “Facile green synthesis of gold nanoparticles with gum arabic as a stabilizing agent and reducing agent,” Gold Bulletin, vol. 43, no. 4, pp. 234–240, 2010.

P. Ravindra, “Protein-mediated synthesis of gold nanoparticles,” Materials Science and Engineering: B Advanced Functional Solid-State Materials, vol. 163, no. 2, pp. 93–98, 2009.

A. Akhavan, H. R. Kalhor, M. Z. Kassaee, N. Sheikh, and M. Hassanlou, “Radiation synthesis and characterization of protein stabilized gold nanoparticles,” Chemical Engineering Journal, vol. 159, no. 1-3, pp. 230–235, 2010.

M. P. Neupane, S. J. Lee, I. S. Park et al., “Synthesis of gelatin-capped gold nanoparticles with variable gelatin concentration,” Journal of Nanoparticle Research, vol. 13, no. 2, pp. 491–498, 2011.

S. Nath, C. Kaittanis, A. Tinkham, and J. M. Perez, “Dextran-coated gold nanoparticles for the assessment of antimicrobial susceptibility,” Analytical Chemistry, vol. 80, no. 4, pp. 1033–1038, 2008.

Z. Gao, R. Su, R. Huang, W. Qi, and Z. He, “Glucomannan-mediated facile synthesis of gold nanoparticles for catalytic reduction of 4-nitrophenol,” Nanoscale Research Letters, vol. 9, no. 1, pp. 1–8, 2014.

M.-C. Daniel and D. Astruc, “Gold nanoparticles: assembly, supramolecular chemistry, quantum-size-related properties, and applications toward biology, catalysis, and nanotechnology,” Chemical Reviews, vol. 104, no. 1, pp. 293–346, 2004.

S. F. Chen, J. P. Li, K. Qian et al., “Large scale photochemical synthesis of M@TiO₂ nanocomposites (M = Ag, Pd, Au, Pt) and their optical properties, CO oxidation performance, and antibacterial effect,” Nano Research, vol. 3, no. 4, pp. 244–255, 2010.

Z. Nie, K. J. Liu, C.-J. Zhong et al., “Enhanced radical scavenging activity by antioxidant-functionalized gold nanoparticles: A novel inspiration for development of new artificial antioxidants,” Free Radical Biology & Medicine, vol. 43, no. 9, pp. 1243–1254, 2007.

C. D. Medley, J. E. Smith, Z. Tang, Y. Wu, S. Bamrungsap, and W. Tan, “Gold nanoparticle-based colorimetric assay for the direct detection of cancerous cells,” Analytical Chemistry, vol. 80, no. 4, pp. 1067–1072, 2008.

S. A. C. Carabineiro, N. Bogdanchikova, A. Pestryakov, P. B. Tavares, L. S. G. Fernandes, and J. L. Figueiredo, “Gold nanoparticles supported on magnesium oxide for CO oxidation,” Nanoscale Research Letters, vol. 6, article no. 435, pp. 1–6, 2011.

M. Chandra and P. K. Das, “Green routes to noble metal nanoparticle synthesis,” International Journal of Green Nanotechnology: Physics and Chemistry, vol. 1, no. 1, pp. P10–P25, 2009.

A. N. de Belder, “Dextran, Industrial gums: polysaccharides and their derivatives,” in A. N. de Belder, R. L. Whistler and J. L. BeMiller, Eds., pp. 399–425, Academic Press, 1993.

A. N. de Belder, “Medical applications of dextran and its derivative, polysaccharides in medicinal applications,” in A. N. de Belder, S. Dumitriu, Ed., pp. 505–523, Marcel Dekker, New York, NY, USA, 1996.

K. P. Bankura, D. Maity, M. M. R. Mollick et al., “Synthesis, characterization and antimicrobial activity of dextran stabilized silver nanoparticles in aqueous medium,” Carbohydrate Polymers, vol. 89, no. 4, pp. 1159–1165, 2012.

J. F. Hainfeld, D. N. Slatkin, T. M. Focella, and H. M. Smilowitz, “Gold nanoparticles: a new X-ray contrast agent,” British Journal of Radiology, vol. 79, no. 939, pp. 248–253, 2006.

O. S. Muddineti, B. Ghosh, and S. Biswas, “Current trends in using polymer coated gold nanoparticles for cancer therapy,” International Journal of Pharmaceutics, vol. 484, no. 1-2, pp. 252–267, 2015.

R. Geetha, T. Ashokkumar, S. Tamilselvan, K. Govindaraju, M. Sadiq, and G. Singaravelu, “Green synthesis of gold nanoparticles and their anticancer activity,” Cancer Nanotechnology, vol. 4, no. 4-5, pp. 91–98, 2013.

Y. Ren, H. Qi, Q. Chen, and L. Ruan, “Thermal dosage investigation for optimal temperature distribution in gold nanoparticle enhanced photothermal therapy,” International Journal of Heat and Mass Transfer, vol. 106, pp. 212–221, 2017.

C. Yao, L. Zhang, J. Wang et al., “Gold nanoparticle mediated phototherapy for cancer,” Journal of Nanomaterials, vol. 2016, Article ID 5497136, 29 pages, 2016.

D. V. Phu, V. T. K. Lang, N. T. K. Lan et al., “Synthesis and antimicrobial effects of colloidal silver nanoparticles in chitosan by γ-irradiation,” Journal of Experimental Nanoscience, vol. 5, no. 2, pp. 169–179, 2010.

L. Huang, M. Zhai, J. Peng, L. Xu, J. Li, and G. Wei, “Synthesis, size control and fluorescence studies of gold nanoparticles in carboxymethylated chitosan aqueous solutions,” Journal of Colloid and Interface Science, vol. 316, no. 2, pp. 398–404, 2007.

K. Makuuchi, An introduction to radiation vulcanization of natural rubber latex, T.R.I. Global Co. Ltd, Bangkok, Thailand, 2003.

S. K. Balasubramanian, L. Yang, L.-Y. L. Yung, C.-N. Ong, W.-Y. Ong, and L. E. Yu, “Characterization, purification, and stability of gold nanoparticles,” Biomaterials, vol. 31, no. 34, pp. 9023–9030, 2010.

ISO 11137 – 2:2013, Sterilization of health care products – Radiation – Part 2: Establishing the sterilization dose.